Microstructure evolution and mechanical performance of ... Microstructure evolution and mechanical...
Embed Size (px)
Transcript of Microstructure evolution and mechanical performance of ... Microstructure evolution and mechanical...
Contents lists available at ScienceDirect
journal homepage: www.elsevier.com/locate/matchar
Microstructure evolution and mechanical performance of copper processed by equal channel angular rolling
T. Kvackaja, A. Kovacovaa, R. Kociskoa, J. Bidulskaa, L. Lityńska–Dobrzyńskab, P. Jeneic, J. Gubiczac,⁎
a Faculty of Metallurgy, Technical University of Košice, Letna 9, 04200 Kosice, Slovakia b Institute of Metallurgy and Materials Science of the Polish Academy of Science, Krakow, Poland c Department of Materials Physics, ELTE Eötvös Loránd University, Budapest, Hungary
A R T I C L E I N F O
Keywords: Equal channel angular rolling (ECAR) Ultrafine-grained copper Microstructure Dislocation density Mechanical properties
A B S T R A C T
Ultrafine-grained (UFG) oxygen free high conductivity (OFHC) Cu samples were processed by severe plastic deformation (SPD) using the method of equal channel angular rolling (ECAR) up to 33 passes at room tem- perature. It was found that the grain size gradually decreased from ~40 μm to ~250 nm with increasing the number of passes. A maximum dislocation density of ~21 × 1014 m−2 was achieved after 13 passes of ECAR. For large numbers of passes (between 23 and 33), the dislocation density decreased to ~14 × 1014 m−2. The proof stress was saturated at the value of about 400 MPa. The stored energy was measured by calorimetry and compared with the values calculated from the parameters of the microstructure. The reduction of the released heat after 13 and 33 passes suggested structural relaxation of the UFG microstructure. For these numbers of passes, the reduction of area in tensile testing was improved without decreasing the proof stress. The correlation between the microstructure and the mechanical behavior was discussed in detail. It was found that ECAR is capable for the mass-production of UFG metallic materials with high strength, therefore this method is a possible way of commercialization of SPD-processed materials.
Porosity and contamination-free, high strength metallic materials can be produced by severe plastic deformation (SPD) procedures [1–3]. Applying these methods, the elevated mechanical strength is achieved via the refinement of the grain structure into the ultrafine-grained (UFG) regime and the increase of the dislocation density to extremely high values . Numerous SPD procedures were developed in the last decades, such as equal channel angular pressing (ECAP) [5–8], high- pressure torsion (HPT) , multi-directional forging (MDF) , twist extrusion (TE) [3,11] and accumulative roll-bonding (ARB) . Al- though, these methods yield UFG metallic materials with high strength, they are not suitable for mass-production due to the very limited di- mensions of the as-processed workpieces.
Efforts were made in the literature to develop SPD procedures which are capable to process large amounts of UFG materials in a reasonable time. For instance, the classical ECAP technique was modified in order to provide a solution for the continuous production of UFG materials which is referred to as ECAP-Conform process . Another candidate for mass-production of UFG metals is equal channel angular rolling
(ECAR) which combines rolling and ECAP steps in materials processing . First, the workpiece is rolled and then the specimen passed be- tween the rolls is introduced into an ECAP die. This process can be carried out either on large, thin sheets or long, rod-like samples. In the last decade, ECAR-processing was successfully applied on pure Cu [13,14], Al-alloys such as Al 5083 , Al 1100 , Al 7050 , Mg-alloys such as AZ31 [18–20] and bimetal Al/Cu sheets . It was shown that ECAR resulted in a significant grain refinement for all me- tallic materials. For instance, in AZ31 alloys the initial grain size of ~20 μm was reduced to about 30 nm after 10 passes of ECAR . The significant grain refinement yielded a considerable increase in strength and hardness. It seems that the majority of grain refinement and hardness increment occurred during the first pass of ECAR . The ductility usually decreases for ECAR-processed materials due to the loss of the strain hardening capability . At the same time, for AZ31 alloy the drawability was improved by ECAR owing to the variation of the deformation mechanisms as a result of the change in the crystal- lographic texture [18,19]. For precipitation-hardened Al-alloys, ECAR- processing led to a fragmentation of plate-like precipitates into sphe- rical particles which also influences the hardness . It was shown
http://dx.doi.org/10.1016/j.matchar.2017.10.030 Received 28 August 2017; Received in revised form 30 October 2017; Accepted 30 October 2017
⁎ Corresponding author. E-mail address: email@example.com (J. Gubicza).
Materials Characterization 134 (2017) 246–252
Available online 31 October 2017 1044-5803/ © 2017 Elsevier Inc. All rights reserved.
http://www.sciencedirect.com/science/journal/10445803 https://www.elsevier.com/locate/matchar http://dx.doi.org/10.1016/j.matchar.2017.10.030 http://dx.doi.org/10.1016/j.matchar.2017.10.030 mailto:firstname.lastname@example.org http://dx.doi.org/10.1016/j.matchar.2017.10.030 http://crossmark.crossref.org/dialog/?doi=10.1016/j.matchar.2017.10.030&domain=pdf
that ECAR-processing of Cu strips at room temperature (RT) led to a high strength of about 300 MPa and a reduced elongation to failure (about 6%) . In that work, the maximum number of passes was eight. It was also revealed that short time annealing after ECAR-pro- cessing may yield a slight improvement in strength, ductility and con- ductivity due to partial recrystallization. Other work  has shown that the application of ECAR on a Cu bar with rectangular cross section can yield a very large strength of about 400 MPa. In these experiments, ECAR deformation was performed only up to 13 passes.
The goal of this study is to investigate the microstructure, the thermal stability and the mechanical behavior of ECAR-processed Cu. The results obtained on the specimens processed by ECAR are compared with the properties of ECAP-processed Cu samples as ECAR is suitable for mass production while ECAP is mainly a laboratory technique. Former studies on ECAP-processed Cu have shown that deformation up to very high numbers of passes (16–25 passes [22,23]) can result in a structural relaxation which may improve the ductility of the UFG Cu specimens. Similar study on ECAR-processed Cu is missing from the literature. Therefore, the present study was extended to 33 passes of ECAR. The microstructure was studied by transmission electron mi- croscopy (TEM) and X-ray line profile analysis (XLPA). The latter method enables the determination of the density and arrangement of dislocations with good statistics. Our study is unique in the literature as the dislocation structure in ECAR-processed Cu has not been studied yet. In addition, the energy stored in the lattice defect structure was determined by calorimetry as a function of the number of passes. The correlation between the mechanical performance and the micro- structure was discussed in detail.
2. Experimental Material and Methods
The initial material was oxygen free high conductivity copper (OFHC with the purity of 99.99%). The grain size and the mechanical properties of the initial OFHC Cu are given in Table 1. The initial Cu samples were processed by zonal refining and cold drawing with an elongation of 200%. Then, the specimens were subjected to one pass of caliber rolling before their entering the ECAR channel. The schematic of the ECAR facility is shown in Fig. 1. Specimens were processed by ECAR with a die channel angle of Φ= 90° at RT. Before ECAR, the samples have a rectangular cross section with the dimension of 7 × 6 mm2 and a length of 500 mm. The ECAR process was carried out using a duo rolling mill with rolls diameter of D = 210 mm. The pressing velocity during ECAR was 0.2 mm/s. Route A was applied, i.e., the samples were not rotated between the subsequent passes. The maximum number of ECAR passes was 33. Finite element modeling (not shown here) re- vealed that the temperature of the specimens during ECAR increased to about 90 °C. The microstructure and the mechanical behavior were studied as a function of the numbers of ECAR passes. The micro- structure was investigated by TEM using a Philips CM20 microscope. The surface of the TEM foil was parallel to plane x-z shown in Fig. 1. It is noted that in order to avoid any recovery and recrystallization during the study of the severely deformed microstructures, the ECAR-pro- cessed samples were stored in a freezer.
The microstructure of the specimens was also studied by XLPA. The X-ray line profiles were measured by a high-resolution rotating anode diffractometer (Rigaku, RA Multimax9) using CuKα1 (λ = 0.15406 nm)
radiation. The Debye–Scherrer diffraction rings were detected by two dimensional imaging plates and the line profiles were determined as the intensity distributions perpendicular to the rings obtained by in- tegrating the two dimensional intensity distributions along the rings. The evaluation of the patterns was carried out by the Convolutional Multiple Whole Profile (CMWP) fitting method . In this procedure, the experimental diffraction pattern is fitted by the sum of a back- ground spline and the convolution of the instrumental pattern and the theoretical line profiles related to crystallite size, dislocations and planar faults. The theoretical line profile functions used in this fitting procedure were based on a model of the microstructure where the crystallites have spherical shape and a log-no